EPJ Photovoltaics 9, 3 (2018) © X. Zhang et al., published by EDP Sciences, 2018 https://doi.org/10.1051/epjpv/2018002
EPJ Photovoltaics Available online at: www.epj-pv.org
Chalcogenide glass-ceramic with self-organized heterojunctions: application to photovoltaic solar cells Xianghua Zhang1, Ilia Korolkov1, Bo Fan1, Michel Cathelinaud1,*, Hongli Ma1, Jean-Luc Adam1, Odile Merdrignac1, Laurent Calvez1, Hervé Lhermite2, Laurent Le Brizoual2, Marcel Pasquinelli3, and Jean-Jacques Simon3 1 2 3
Univ. Rennes, CNRS, ISCR –UMR6226, 35000 Rennes, France Univ. Rennes, CNRS, IETR –UMR6164, 35000 Rennes, France Aix Marseille Université, CNRS, Université de Toulon, IM2NP UMR 7334, 13397 Marseille, France Received: 31 January 2017 / Received in ﬁnal form: 25 September 2017 / Accepted: 10 January 2018 Abstract. In this work, we present for the ﬁrst time the concept of chalcogenide glass-ceramic for photovoltaic applications with the GeSe2–Sb2Se3–CuI system. It has been demonstrated that thin ﬁlms, deposited with the sputtering technique, are amorphous and can be crystallized with appropriate heat treatment. The thin ﬁlm glassceramic behaves as a p-type semiconductor, even if it contains p-type Cu2GeSe3 and n-type Sb2Se3. The conductivity of Sb2Se3 has been greatly improved by appropriate iodine doping. The ﬁrst photovoltaic solar cells based on the association of iodine-doped Sb2Se3 and the glass-ceramic thin ﬁlms give a short-circuit current density JSC of 10 mA/cm2 and an open-circuit voltage VOC of 255 mV, with a power conversion efﬁciency of about 0.9%. Keywords: chalcogenide / glass-ceramics / photovoltaic solar cells / heterojunction
1 Introduction Glass-ceramics are composite materials containing a mixture of amorphous and crystalline phases. They have been mainly developed for improving the thermomechanical properties of glasses [1–3]. A wide range of products is now commercially available from mirrors for large telescopes to cooking plates. More recently, glass-ceramics have also been intensively studied as highly efﬁcient luminescent materials in order to simultaneously beneﬁt from the advantages of glasses (easy production and shaping) and of crystals (favorable environment of the luminescence of active ions) [4,5]. Chalcogenide glasses are glasses based on chalcogen elements (S, Se and Te) associated with other elements such as Ge, Sb. They are particularly studied for their good transparence in the mid infrared region [6–9]. Glassceramics are generally obtained by controlling the crystallization of the precursor glass through heat treatment. This thermal process is critical for generating appropriate crystalline phases which will determine the properties of the ﬁnal composite material. Our study on the glass forming system GeSe2–Sb2Se3– CuI was motivated by the development of infrared transmission glass-ceramics . Controlled crystallization * e-mail: [email protected]
of selected glasses leads to glass-ceramics containing simultaneously p-type Cu2GeSe3 (bandgap around 0.8 eV) and n-type Sb2Se3 (bandgap between 1.1 and 1.3 eV) semiconducting phases with appropriate bandgap for solar energy harvesting . The high-resolution transmission electron microscope (HRTEM) indicates, in addition, that these two phases are generally assembled, forming therefore a high number of p-n junctions at a nanoscale and leading to some quite exceptional photoelectric properties such as extremely long lifetime of minority charge carriers in the range of 14 ms. Previous studies, mentioned above, have led to an optimized composition of 40GeSe2–40Sb2Se3–20CuI (in molar percentage) with the highest photocurrent. In this work, we have decided to use this composition to demonstrate the feasibility of a new type of thin ﬁlm photovoltaic solar cells by using this glass-ceramic. To the best of our knowledge, this is the ﬁrst time that a glassceramic is proposed for a photovoltaic application.
2 Experimental section 2.1 Glass-ceramic target For the synthesis of chalcogenide glass-ceramics, it is essential to operate in vacuum because of the relatively high vapor pressure of chalcogenide melt and their tendency to react with oxygen, especially at high temper-
This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
X.H. Zhang et al.: EPJ Photovoltaics 9, 3 (2018)
Fig. 1. Schematic illustration of the deposition system where target A is the glass-ceramic GC40–40–20 and target B is Sb2Se3:I. The set-up is equipped with an optical monitoring system by measuring the reﬂectance on substrate C, where the ﬁlm is deposited. The distance between target and substrate is to 55 mm.
atures. Consequently, the glass-ceramic targets have been produced by using the melt-quenching process with the corresponding element mixtures in sealed silica tube under vacuum. This technique is commonly used for chalcogenide glass preparation and has been described in detail elsewhere . The 40GeSe2–40Sb2Se3–20CuI target (GC40–40–20) and the iodine-doped Sb2Se3 targets were prepared using polycrystalline germanium (99.999% Umicore), antimony (99.999% Umicore), selenium (99.999% Umicore), CuI (98% Aldrich) and iodine (99.9% Aldrich) as starting materials which are weighed according to the composition in order to get a sample of about 60 g. The preparation was done in a silica ampoule with 50 mm internal diameter. The tube was cleaned by hydroﬂuoric acid for about 10 s to eliminate possible dust, which can be present on the wall of the silica ampoule. It was then thoroughly rinsed with deionized water and dried under vacuum. A vacuum trap placed in liquid nitrogen is used to condense any volatile products and also to improve the vacuum. All the starting materials were loaded into the silica tube which was then sealed under a typical vacuum of around 10 5 mbar. The tube containing the mixture was put into a rocking furnace and heated to 800 °C at the rate of 1.5 °C/min and hold for about 12 h to ensure a thorough reaction and homogenization. Then the furnace was cooled down to 700 °C and the thermal quenching was performed by putting the sealed tube into water at room temperature. The rapid quenching is necessary to avoid excessive crystal growth. The thermal shock in the quenching process generated high mechanical stresses in the glass-ceramics. In order to reduce these stresses, the targets were annealed at 200 °C for 3 h. The targets were then cooled down slowly and released from the silica ampoule. After the annealing, the two targets: the glass-ceramic GC40–40–20 and the Sb2Se3:I (10 at.% of iodine named Sb2Se3:I10) with diameter of 50 mm were obtained with a thickness approximatively of 4 mm. They will be used as sputtering targets.
2.2 Thin ﬁlm deposition The sputtering technique is a widely used thin ﬁlm deposition method with good composition transfer from the target to the substrates, even in case of complex composition. We use radio-frequency sputtering technique to deposit thin ﬁlm and the equipment is a MP600S from Plassys. To control the thin ﬁlm growth in real time, the deposition facility is equipped with an online optical monitoring system by reﬂection [12–14]. This system is particularly useful for controlling the crystallization of the thin ﬁlms. The ﬁrst step of the thin ﬁlm deposition is to obtain a homogenous amorphous ﬁlm and therefore, a relatively low deposition pressure of 5 10 3 mbar to ensure a high compactness . The deposition chamber was pumped to a residual pressure of less than 2 10 7 mbar before each deposition. All targets are etched by argon plasma during about 5 min to eliminate surface contamination. The RF sputtering powers are ﬁxed to 13 W on a 50 mm diameter target and the obtained DC bias is typically between 83 and 95 volts. The deposition rate is respectively about 4 nm/min and 6 nm/min for GC404020 and Sb2Se3:I. The deposition system is schematically illustrated in Figure 1, with the possibility of using three confocal targets of 50 mm in diameter (only two targets are illustrated for the sake of clarity). The 40GeSe2–40Sb2Se3–20CuI precursor glass and the iodine-doped Sb2Se3 targets were prepared by using the melt-quenching technique discussed above. These two targets are used for the deposition of multilayer structures, necessary for the photovoltaic device. A thermal annealing system is installed to heat the backside of the substrates, during or after the deposition of thin ﬁlms. Commercial ITO (Indium-Tin Oxide of 30 V/sq) coated soda lime glass (1 mm of thickness) has been used in this work. Two gold contacts (2 mm diameter) were deposited through a physical mask at the end with a LEICA DC Sputtering system.
X.H. Zhang et al.: EPJ Photovoltaics 9, 3 (2018)
Fig. 2. The X-ray diffraction pattern and the morphology of crystallized 40GeSe2–40Sb2Se3–20CuI thin ﬁlm. The diffraction peaks can be assigned to the orthorhombic phases for Sb2Se3 (JCPDS 75-1462) and Cu2GeSe3 (JCPDS 85-1699).
2.3 Heat treatment of thin ﬁlms The heat treatment is a critical step to be optimized for obtaining appropriate microstructure of the thin ﬁlms. It can be done, in-situ, during or after the deposition of the ﬁlms by heating the substrate and the crystallization and cooling were monitored by measuring the optical reﬂectance. The pressure during the heat-treatment is low to avoid any contamination. The temperature for the heattreatment is optimized and the best temperature is 400 °C for the GC40–40–20. The ﬁrst criterion to stop heat treatment is based on a fast decrease of the reﬂectance at 790 nm (wavelength used for monitoring), with more than 10% of variation. The second criterion is to observe a stability of reﬂectance when the temperature decreases during the cooling. When these two criteria are satisﬁed, the annealing will be stopped. The duration of the heat treatment is typically between 5 and 60 min for different thin ﬁlms, which crystallize more or less easily. This duration is optimized for each thin ﬁlm. 2.4 Characterization and measurements X-ray diffraction (XRD) was carried out on a PANalytical’s X-ray diffractometer with a step width of 0.02° and a counting duration of 0.13 s/step. The structure of the GC40–40–20 and Sb2Se3:I ﬁlms was investigated by XRD with Cu Ka1 and Cu Ka2 (wavelengths of 0.154060 nm and 0.154443 nm respectively). Scanning electron microscope (SEM) images and energy dispersive spectrometer (EDS) elemental mappings were obtained with a JEOL JSM7100F. Optical reﬂectance was measured by using a Perkin Elmer lambda 900 spectrophotometer. The photovoltaic devices were characterized under an AM1.5G solar simulator with an illumination intensity of 100 mW/cm2 (450 W Oriel, model 9119). The Keithley 2400 was used to measure the current-voltage characteristics. The acquisition scan rate was 0.05 V/s. The device
area (2 mm in diameter) was deﬁned by the size of the gold electrodes. During the measurements, a diaphragm of 2 mm in diameter was placed in front of the plot of gold to illuminate only this plot. No temperature control was applied. A HMS-5000 Hall effect measurement system (Ecopia) was used to measure the concentration and the mobility of the minority charge carriers, the resistivity, the conductivity and the Hall coefﬁcient at room temperature for thin ﬁlms. Photo-electro-chemical (PEC) measurements have been performed by using the classic 3-electrode method. The sample to be measured was used as the working electrode in association with a platinum counter electrode and the Ag/AgCl reference electrode. Aqueous solution of 0.5 M LiClO4 was used as electrolyte. The potential difference was measured between the reference electrode and the working electrode. The current density was measured between the Pt electrode and the working electrode. A potentiostat AUTOLAB METROHM and a chopped white light lamp of 150 W with an intensity of 30 mW/cm2 on the sample were employed to record current-voltage (I-V) characteristics. The result was analyzed by using the NOVA software.
3 Results and discussion Thin ﬁlms deposited with the substrate at room temperature, are conﬁrmed, by XRD, to be amorphous. The asdeposited thin ﬁlms, without annealing, have high electric resistance and no photocurrent can be detected. Optical monitoring indicates that the heat treatment of the precursor amorphous thin ﬁlms is efﬁcient at temperatures higher than 300 °C in order to get crystallized thin ﬁlm of GC404020. The XRD pattern, shown in Figure 2, conﬁrms the presence of the two crystalline phases, Cu2GeSe3 and Sb2Se3, and an amorphous phase like in the bulk glassceramic samples. As discussed before, antimony selenide
X.H. Zhang et al.: EPJ Photovoltaics 9, 3 (2018)
12 Film GC 404020 on ITO
Log (resistivity in .cm)
Current density (µA/cm )
Ligth off 0
Ligth on -400
6 4 2 0 0
Iodine content in Sb2Se3 (mol%)
Fig. 4. Resistivity as function of iodine doping in Sb2Se3. -0,4
Potential applied (V)
Fig. 3. Photo-electro-chemical measurement showing the dark and light current-voltage characteristics of GC 404020 thin ﬁlm, indicating clearly it is a p-type semi-conductor.
(Sb2Se3) has an orthorhombic structure with an optical band gap of 1.1 1.3 eV . The copper germanium selenide (Cu2Ge2Se3) has an optical bandgap of 0.8 eV . The morphology of the ﬁlm is also shown in the same ﬁgure and the needle-like structure of Sb2Se3 can be clearly seen. The PEC measurement (Fig. 3) shown clearly important photocurrent at negative bias, indicating that the crystallized GC40–40–20 thin ﬁlm is a p-type semiconductor. There is an important difference with the bulk glassceramic showing a simultaneous p-type and n-type semiconducting behavior . In fact, in the above mentioned previous study, it has been demonstrated that, in the bulk glass-ceramics, the p-type semiconducting phase is Cu2GeSe3 and the n-type is iodine doped Sb2Se3. Sb2Se3 is a semiconductor with very low conductivity. The iodine doping is essential for improving the conductivity of Sb2Se3, as shown in Figure 4. However, due to its relatively high partial pressure, iodine content will be lower in the thin ﬁlm than in the bulk target. This explains well the different behaviors between bulk and thin ﬁlm in terms of PEC results. As the thin ﬁlm glass-ceramic 40GeSe2–40Sb2Se3– 20CuI is only p-type semiconductor, a n-type semiconductor is necessary to create p-n junctions. It has been demonstrated, by Hall effect measurements and PEC measurements, that iodine-doped Sb2Se3 was a n-type semiconductor with appropriate conductivity. Therefore, Sb2Se3:I thin ﬁlms have been developed with a iodinedoping level of 10 mol%. For the Sb2Se3:I ﬁlm, the heat treatment temperature should be lower to avoid decomposition of this ﬁlm and to limit the loss of iodine. As an example, a heat treatment at 272 °C with a pressure of 0.25 mbar leads to the crystallization of Sb2Se3 without any impurity phase, as shown in Figure 5. The introduction of iodine in Sb2Se3, evidenced by the important increase of conductivity, does not lead to a signiﬁcant shift of the diffraction peaks. This can be attributed to the close radii of Se2 and I ions (respectively 1.98 A and 2.16 A). Iodine doped Sb2Se3 is a ntype semiconductor with a resistivity in the range of
100 V · cm for heat treatment conditions inferior to 272 °C. Above this temperature, the ﬁlms deposited on glass (Bk7 or soda-lime glass) tend to decompose and result in a bad mechanical adhesion on substrate. EDS measurements indicate some losses of selenium and iodine during the thin ﬁlm deposition. Optimized heat treatment does induce noticeable composition change. In view of a different annealing temperatures, the GC40–40–20 ﬁlm should be deposited before the Sb2Se3:I ﬁlm during the preparation of the solar cells. The controlled crystallization has a key impact on the performance of these different materials. The heat treatment is generally realized inside the vacuum chamber after the deposition of each layer by heating the backside of the substrate. It has been observed that a relatively thick ﬁlm will lead to inhomogeneous crystallization. For this reason, we decided to design a PV device with relatively thin ﬁlms. The structure of the photovoltaic device is shown in Figure 6. The choice of the ﬁrst layer deposited on ITO ﬁlm has been ﬁxed in respect with the band gap of thin ﬁlms and the heat treatment conditions. The selected thickness is 220 nm for the layer of Sb2Se3:I and 150 nm for the GC40–40–20 glass-ceramic layer. These thin ﬁlms are heat treated together after the deposition during 40 min at 270 °C. Figure 6 gives also the current-voltage characteristics in dark and under illumination of a solar simulator. This device gives a short-circuit current density JSC of 10 mA/cm2 and an open-circuit voltage VOC of 255 mV. The illumination does not lead to a perfect offset of the I-V curves. The ﬁll factor is 35%, leading to a power conversion efﬁciency of about 0.9%. In order to verify the origin of the photovoltaic effect, two separate junctions, Au/Sb2Se3:I and chalcogenide glass-ceramics/ITO have been fabricated. The I-V characteristic of these two junctions has been measured, indicating clearly two ohmic contacts. Similar results have been obtained with Au/Sb2Se3 junction by another group . Therefore, we can conclude that the photovoltaic effect is induced by the junction chalcogenide glassceramic/Sb2Se3:I. The reproducibility of this device has been tested with similar results: The short-circuit current density is typically in the range of 9–10 mA/cm2 and more variation for the VOC has been observed in the range of 230–280 mV.
X.H. Zhang et al.: EPJ Photovoltaics 9, 3 (2018)
Fig. 5. XRD pattern of Sb2Se3:I ﬁlm on BK7 after heat treatment at 272 °C. The diffraction peaks can be assigned to the orthorhombic phases for Sb2Se3 (JCPDS 75-1462).
Fig. 6. The schematized structure and the I-V characteristics of the photovoltaic device using chalcogenide glass-ceramics.
4 Conclusion and perspectives In this work, we have demonstrated the feasibility of GeSe2–Sb2Se3–CuI thin ﬁlm with controlled crystallization by using the sputtering technique. The XRD has conﬁrmed the co-existence of Cu2GeSe3 with the Sb2Se3 in the partially crystallized thin ﬁlm as in the previously studied bulk glass-ceramics. The thin ﬁlm shows only a p-type semiconductor behaviors, while the bulk glass-ceramics show simultaneous p-type and n-type characteristics. Therefore, a n-type semiconductor has been developed by doping Sb2Se3 with iodine, leading to considerably decreased resistivity of Sb2Se3. Photovoltaic devices have been fabricated based on the chalcogenide glass-ceramics associated with the iodinedoped Sb2Se3 which is a n-type semiconductor. For this totally new type of solar cells, an interesting Jsc of 10 mA/cm2 before any optimization has been reproducibly obtained with a very thin absorber layer. The power
conversion efﬁciency is about 1%. The structure and the absorber’s thickness should be optimized in order to increase the power conversion efﬁciency of this photovoltaic device using totally new materials.
References 1. G. Partridge, Glass Technol. 35, 116 (1994) 2. D.S. Baik, K.S. No, J.S.S. Chun, J. Am. Ceram. Soc. 78, 1217 (1995) 3. H.L. Ma, X.H. Zhang, J. Lucas, J. Non-Cryst. Solids 317, 270 (2003) 4. M. Takahashi, M. Izuki, R. Kanno, Y. Kawamoto, J. Appl. Phys. 83, 3920 (1998) 5. Q. Luo, X.S. Qiao, X.P. Fan, H.Y. Fu, J.L. Huang, Y.J. Zhang, B. Fan, X.H. Zhang, J. Am. Ceram. Soc. 95, 1042 (2012) 6. C.D. Hwan, K.H. Jeong, H. Yeon et al., Appl. Opt. 51, 5649 (2012)
X.H. Zhang et al.: EPJ Photovoltaics 9, 3 (2018)
7. Chalcogenide glasses, preparation, properties and applications, edited by J.L. Adam, X. Zhang (Woodhead Publishing, 2013) 8. A. Yang, M. Zhang, L. Li et al., J. Am. Ceram. Soc. 99, 12 (2016) 9. X.H. Zhang, Y. Guimond, Y. Bellec, J. Non-Cryst. Solids 326 & 327, 519 (2003) 10. L. Calvez, H.L. Ma, J. Lucas, X.H. Zhang, Phys. Chem. Glasses Eur. J. Glass Sci Technol. B 47, 142 (2006) 11. X.H. Zhang, Y. Xu, Q. Shen, B. Fan, X. Qiao, X. Fan, H. Yang, Q. Luo, L. Calvez, H.L. Ma, M. Cathelinaud, J.J. Simon, J. Mater. Chem. A 2, 17099 (2014) 12. B. Badoil, F. Lemarchand, M. Cathelinaud, M. Lequime, Opt. Express 16, 12008 (2008)
13. W. Shen, M. Cathelinaud, M. Lequime, F. Charpentier, V. Nazabal, Opt. Express 16, 373 (2008) 14. V. Nazabal, M. Cathelinaud, W. Shen, P. Nemec, F. Charpentier, H. Lhermite, M.L. Anne, J. Capoulade, F. Grasset, A. Moreac, S. Inoue, M. Frumar, J.L. Adam, M. Lequime, C. Amra, Appl. Opt. 47, C114 (2008) 15. J.A. Thornton, J Vac. Sci. Technol. A 4, 3059 (1986) 16. G.H. Liang, Z.H. Zheng, P. Fan, J.T. Luo, J.G. Hu, X.H. Zhang, H.L. Ma, B. Fan, Z.K. Luo, D.P. Zhang, Sol Energy Mater. Sol. Cells 174, 263 (2018) 17. B.K. Sarkar, A.S. Verma, P.S. Deviprasad, Physica B 406, 2847 (2011) 18. C. Chen, D.C. Bobela, Y. Yang, S.C. Lu, K. Zeng, C. Ge, B. Yang, L. Gao, Y. Zhao, M.C. Beard, J. Tang, Front Optoelectron. 10, 18 (2017)
Cite this article as: Xianghua Zhang, Ilia Korolkov, Bo Fan, Michel Cathelinaud, Hongli Ma, Jean-Luc Adam, Odile Merdrignac, Laurent Calvez, Hervé Lhermite, Laurent Le Brizoual, Marcel Pasquinelli, Jean-Jacques Simon, Chalcogenide glass-ceramic with self-organized heterojunctions: application to photovoltaic solar cells, EPJ Photovoltaics 9, 3 (2018)